Presentation on theme: "MASS TRANSFER IN MEMBRANE PROCESSES"— Presentation transcript:
1MASS TRANSFER IN MEMBRANE PROCESSES SEPARATIONMASS TRANSFER IN MEMBRANE PROCESSES
2Permeation mechanism model TRANSPORT MODELSMembrane selective : Ability to control the rate of permeation of different speciesbased on pore sizePore-flow/sieving modelPermeants are transported by pressure-driven convective flow through tiny poresSeparation occurs because one of the permeants is excluded (filtered) from some of the pores in the membrane through which other permeants moveThe free-volume elements (pores) are relatively large and fixed, do not fluctuate in position or volume on the timescale of permeant motion, and are connected to one anotherPermeation mechanism model = 5-10ÅSolution-diffusion modelPermeants dissolve in the membrane material and then diffuse through the membrane down a concentration gradientThe permeants are separated because of the differences in the solubilities of the materials in the membrane and the differences in the rates at which the materials diffuse through the membraneThe free-volume elements (pores) in the membrane are tiny spaces between polymer chains caused by thermal motion of the polymer molecules
3BASIC KNOWLEDGE Diffusion: Solubility: is the process by which matter is transported from one part of a system to another by a concentration gradient … slow process … kinetic parametersimple statistics show that a net transport of matter will occur from the high concentration to the low concentration regionFick‘s lawHigh transport (flux) : thin layer and high concentration differenceSolubility:A thermodynamic parameter and gives a measure of the amount of permeants/penetrant sorbed by the membrane under equilibrium conditionsSolubility of gas ... Henry‘s lawPermeability (P) = Solubility (S) x Diffusivity (D)For dense/non-porous membranes, e.g. GS, PV, RO, etc.
4Pore-flow vs. Solution diffusion ... Membrane pore size BASIC KNOWLEDGEPore-flow model:Pressure driven convective flowIn capillary or porous mediumDarcy‘s Lawdp/dx : is the pressure gradient existing in the porous mediumCi : is the concentration of component i in the mediumK’ : is a coefficient reflecting the nature of the mediumFluxes obtained is higher compared to simple diffusionThe average pore diameter in a membrane is difficult to be measured directly and must often be inferred from the size of the molecules that permeate the membrane or by some other indirect techniquePore-flow vs. Solution diffusion ... Membrane pore size
5BASIC KNOWLEDGEUF, MF and microporous Knudsen flow gas separation membrane are clearly microporous ... pore flowRO, PV, GS ... a dense polymer layer with no visible pores ... for molecule 2-5ÅNF, fine microporous ... intermediate between truly microporous and truly solution diffusion membranes … for di/trisaccharised (10-13 Å) rejection but freely pass monosaccharides (5-6 Å)Figure : Schematic representation of the nominal pore size and best theoretical model for the principal membrane separation processes
6SOLUTION-DIFUSSION MODEL Molecular Dynamics SimulationsReverse osmosisPervaporationGas Separationuses a large pressure difference across the membrane to separate water from salt solutionsthe pressure difference across the membrane is small, and the process is driven by the vapor pressure difference between the feed liquid and the low partial pressure of the permeate vaportransport of gases down a pressure or concentrationgradientDiffusion processThe pressure, temperature, and composition of the fluids determines the concentration of the diffusing species at the membrane surface in equilibrium with the fluidOnce dissolved in the membrane, individual permeating molecules move by the same random process of molecular diffusion no matter whether the membrane is being used in reverse osmosis, pervaporation, or gas permeation … similar membranes are used in very different processesThe movement or diffusion of individual molecule in free volume (voulme between polymer chain) can be calculated/studied by computer molecular dynamics simulationMolecular dynamics simulations also allow the transition from the solution diffusion to the pore-flow transport mechanism to be seen
7SOLUTION-DIFUSSION MODEL Molecular Dynamics Simulations: example resultDuring the first 100 ps of the simulation, the carbon dioxide molecule bounces around in the cavity where it has been placed, never moving more than about 5 Å , the diameter of the cavity.After 100 ps, however, a chance thermal motion moves a segment of the polymer chains sufficiently for the carbon dioxide Molecule to jump approximately 10 Å to an adjacent cavity where it remains until another movement of the polymer chains allows it to jump to another cavity.By repeating these calculations many times and averaging the distance moved by the gas molecule, its diffusion coefficient can be calculated.far from matching the experimental values ... the best quantitative description of permeation uses phenomenological equations, particularly Fick’s law
8SOLUTION-DIFUSSION MODEL Concentration and Pressure Gradients in MembranesMathematical description of diffusion in membranes based on thermodynamic: the driving forces of pressure, temperature, concentration, and electrical potential are interrelated and that the overall driving force producing movement of a permeant is the gradient in its chemical potentialwhere di/dx is the chemical potential gradient of component i and Li is a coefficient of proportionality (not necessarily constant) linking this chemical potential driving force to flux.Restricting the approach to driving forces generated by concentration and pressure gradients, the chemical potential is written aswhere ni is the mole fraction (mol/mol) of component i, i is the activity coefficient (mol/mol) linking mole fraction with activity, p is the pressure, and i is the molar volume of component i.For incompressible fluid, volume does not change with pressure, thuswhere μio is the chemical potential of pure i at a reference pressure, piO .
9SOLUTION-DIFUSSION MODEL Concentration and Pressure Gradients in MembranesFor incompressible fluid, volume does not change with pressure, thuswhere μio is the chemical potential of pure i at a reference pressure, piO.For compressible fluid, volume does change with pressure, thusreference pressure, piO is defined as the saturation vapor pressure of i, pisat, therefore,for incompressiblefor compressibleAssumptionsThe fluids on either side of the membrane are in equilibrium with the membrane material at the interfaceWhen pressure is applied across a dense membrane, the pressure throughout the membrane is constant at the highest valueThe pressure within a membrane is uniform and that the chemical potential gradient across the membrane is expressed only as a concentration gradient
10SOLUTION-DIFUSSION MODEL Concentration and Pressure Gradients in MembranesPressure driven permeation of a one-component solution through a membrane according to the solution-diffusion transport model𝑐 𝑖 : concentration (g/cm3)𝑚 𝑖 : the molecular weight of I (g/mol)𝜌 : the molar density (mol/cm3)o and l represent the position of the feed and permeate interfaces~ Fick‘s law
11SOLUTION-DIFUSSION MODEL Concentration and Pressure Gradients in Membranes
12PORE FLOW MODELLack of pore flow model ... extremely heterogeneous nature of microporous membranesMolecular sievingBoth methodsdepth filter which captures particles within the interior of the membrane by adsorptionMolecular sieving(a) Nuclepore (polycarbonate) nucleation track membrane; (b) Celgard® (polyethylene) expanded film membrane; (c) Millipore cellulose acetate/cellulose nitrate phase separation membrane made by water vapor imbibition (Courtesy of Millipore Corporation, Billerica, MA); (d) anisotropic polysulfone membrane made by the Loeb–Sourirajan phase separation process … all have app. similar particle rejection
13PORE FLOW MODEL Lack of pore flow model ... Reasons Pore structure Membrane materialCharacterizationPorosity (ε) is the fraction of the total membrane volume that is porousThe membrane tortuosity (τ ) reflects the actual length of the average pore compared to the membrane thicknesspore diameter
14PORE FLOW MODELPermeation in Ultrafiltration and Microfiltration MembranesContain surface pores smaller than the particles to be removedAnisotropicCapture and accumulated on the surfaceCaptures the parti-cles to be removed in the interior of the membraneIsotropicConstrictions and adsorption
15PORE FLOW MODEL Screen filtration The area, A, of the pore available for solute transportto account for the parabolic velocity profile of the fluid as it passes through the poreFerry-Renkin equationCo and Cp are solute concentration in feed and permeate, respectivelyPores are assumed to be equal circular capillaries with a large radius (r)Solvent can freely pass through the pores